# Ring-opening polymerization

   A polymerization in which a cyclic monomer yields a monomeric unit which is acyclic or contains fewer cycles than the monomer. Note: If monomer is polycyclic, the opening of a single ring is sufficient to classify the reaction as ring-opening polymerization.
   Modified from the earlier definition.
In polymer chemistry, ring-opening polymerization (ROP) is a form of chain-growth polymerization in which the terminus of a polymer chain attacks cyclic monomers to form a longer polymer (see figure). The reactive center can be radical, anionic or cationic.
Ring-opening of cyclic monomers is often driven by the relief of bond-angle strain. Thus, as is the case for other types of polymerization, the enthalpy change in ring-opening is negative. Many rings undergo ROP.

## Monomers

Many cyclic monomers are amenable to ROP. These include epoxides, cyclic trisiloxanes, some lactones and lactides, cyclic anhydrides, cyclic carbonates, and amino acid N-carboxyanhydrides. Many strained cycloalkenes, e.g norbornene, are suitable monomers via ring-opening metathesis polymerization. Even highly strained cycloalkane rings, such as cyclopropane and cyclobutane derivatives, can undergo ROP.

## History

Ring-opening polymerization has been used since the beginning of the 1900s to produce polymers. Synthesis of polypeptides which has the oldest history of ROP, dates back to the work in 1906 by Leuchs. Subsequently, the ROP of anhydro sugars provided polysaccharides, including synthetic dextran, xanthan gum, welan gum, gellan gum, diutan gum, and pullulan. Mechanisms and thermodynamics of ring-opening polymerization were established in the 1950s. The first high-molecular weight polymers (M$_n$ up to 10$^5$) with a repeating unit were prepared by ROP as early as in 1976.
New research shows that ROP can be completed with cyclic esters with minimal to no use of solvents by using resonant acoustic mixing.
An industrial application is the production of nylon-6 from caprolactam.

## Mechanisms

Ring-opening polymerization can proceed via radical, anionic, or cationic polymerization as described below. Additionally, radical ROP is useful in producing polymers with functional groups incorporated in the backbone chain that cannot otherwise be synthesized via conventional chain-growth polymerization of vinyl monomers. For instance, radical ROP can produce polymers with ethers, esters, amides, and carbonates as functional groups along the main chain.

### Anionic ring-opening polymerization (AROP)

Anionic ring-opening polymerizations (AROP) involve nucleophilic reagents as initiators. Monomers with a three-member ring structure - such as epoxides, aziridines, and episulfides - undergo anionic ROP.
A typical example of anionic ROP is that of ε-caprolactone, initiated by an alkoxide.

### Cationic ring-opening polymerization

Cationic initiators and intermediates characterize cationic ring-opening polymerization (CROP). Examples of cyclic monomers that polymerize through this mechanism include lactones, lactams, amines, and ethers. CROP proceeds through an S$_N$1 or S$_N$2 propagation, chain-growth process. The mechanism is affected by the stability of the resulting cationic species. For example, if the atom bearing the positive charge is stabilized by electron-donating groups, polymerization will proceed by the S$_N$1 mechanism. The cationic species is a heteroatom and the chain grows by the addition of cyclic monomers thereby opening the ring system.
The monomers can be activated by Bronsted acids, carbenium ions, onium ions, and metal cations.
CROP can be a living polymerization and can be terminated by nucleophilic reagents such as phenoxy anions, phosphines, or polyanions. When the amount of monomers becomes depleted, termination can occur intra or intermolecularly. The active end can "backbite" the chain, forming a macrocycle. Alkyl chain transfer is also possible, where the active end is quenched by transferring an alkyl chain to another polymer.

### Ring-opening metathesis polymerization

Ring-opening metathesis polymerisation (ROMP) produces unsaturated polymers from cycloalkenes or bicycloalkenes. It requires organometallic catalysts.
The mechanism for ROMP follows similar pathways as olefin metathesis. The initiation process involves the coordination of the cycloalkene monomer to the metal alkylidene complex, followed by a [2+2] type cycloaddition to form the metallacyclobutane intermediate that cycloreverts to form a new alkylidene species.
Commercially relevant unsaturated polymers synthesized by ROMP include polynorbornene, polycyclooctene, and polycyclopentadiene.

## Thermodynamics

The formal thermodynamic criterion of a given monomer polymerizability is related to a sign of the free enthalpy (Gibbs free energy) of polymerization: $\Delta G_{p}(xy)=\Delta H_{p}(xy)-T\Delta S_{p}(xy)$ where:
    x and y indicate monomer and polymer states, respectively (x and/or y = l (liquid), g (gaseous), c (amorphous solid), c' (crystalline solid), s (solution));
    ΔH$_p$(xy) is the enthalpy of polymerization (SI unit: joule per kelvin);
    ΔS$_p$(xy) is the entropy of polymerization (SI unit: joule);
    T is the absolute temperature (SI unit: kelvin).
The free enthalpy of polymerization (ΔG$_p$) may be expressed as a sum of standard enthalpy of polymerization (ΔG$_p$°) and a term related to instantaneous monomer molecules and growing macromolecules concentrations: $\Delta G_{p}=\Delta G_{p}^{\circ }+RT\ln {\frac {[\ldots -({\ce {m}})_{i+1}{\ce {m}}^{\ast }]}{[{\ce {M}}][\ldots -({\ce {m}})_{i}{\ce {m}}^{\ast }]}}$ where:
    R is the gas constant;
    M is the monomer;
    (m)$_i$ is the monomer in an initial state;
    m$^*$ is the active monomer.
Following Flory–Huggins solution theory that the reactivity of an active center, located at a macromolecule of a sufficiently long macromolecular chain, does not depend on its degree of polymerization (DP$_i$), and taking in to account that ΔG$_p$° = ΔH$_p$° − TΔS$_p$° (where ΔH$_p$° and ΔS$_p$° indicate a standard polymerization enthalpy and entropy, respectively), we obtain:
    $\Delta G_{p}=\Delta H_{p}^{\circ }-T(\Delta S_{p}^{\circ }+R\ln[M])$
At equilibrium (ΔG$_p$ = 0), when polymerization is complete the monomer concentration ([M]$_{eq}$) assumes a value determined by standard polymerization parameters (ΔH$_p$° and ΔS$_p$°) and polymerization temperature: ${\begin{aligned}[{\ce {M}}]_{\rm {eq}}&=\exp \left({\frac {\Delta H_{p}^{\circ }}{RT}}-{\frac {\Delta S_{p}^{\circ }}{R}}\right)\\[4pt]\ln {\frac {DP_{n}}{DP_{n}-1}}[{\ce {M}}]_{\rm {eq}}&={\frac {\Delta H_{p}^{\circ }}{RT}}-{\frac {\Delta S_{p}^{\circ }}{R}}\\[4pt][{\ce {M}}]_{\rm {eq}}&={\frac {DP_{n}-1}{DP_{n}}}\exp \left({\frac {\Delta H_{p}^{\circ }}{RT}}-{\frac {\Delta S_{p}^{\circ }}{R}}\right)\end{aligned}}$ Polymerization is possible only when [M]$_0$ > [M]$_{eq}$. Eventually, at or above the so-called ceiling temperature (T$_c$), at which [M]$_{eq}$ = [M]$_0$, formation of the high polymer does not occur. ${\begin{aligned}T_{c}&={\frac {\Delta H_{p}^{\circ }}{\Delta S_{p}^{\circ }+R\ln[{\ce {M}}]_{0}}};\quad (\Delta H_{p}^{\circ }<0,\ \Delta S_{p}^{\circ }<0)\\[4pt]T_{f}&={\frac {\Delta H_{p}^{\circ }}{\Delta S_{p}^{\circ }+R\ln[{\ce {M}}]_{0}}};\quad (\Delta H_{p}^{\circ }>0,\ \Delta S_{p}^{\circ }>0)\end{aligned}}$ For example, tetrahydrofuran (THF) cannot be polymerized above T$_c$ = 84 °C, nor cyclo-octasulfur (S$_8$) below T$_f$ = 159 °C. However, for many monomers, T$_c$ and T$_f$, for polymerization in the bulk, are well above or below the operable polymerization temperatures, respectively. The polymerization of a majority of monomers is accompanied by an entropy decrease, due mostly to the loss in the translational degrees of freedom. In this situation, polymerization is thermodynamically allowed only when the enthalpic contribution into ΔG$_p$ prevails (thus, when ΔH$_p$° < 0 and ΔS$_p$° < 0, the inequality |ΔH$_p$| > −TΔS$_p$ is required). Therefore, the higher the ring strain, the lower the resulting monomer concentration at equilibrium.

## Additional reading

* Luck, Russel M.; Sadhir, Rajender K., eds. (1992). Expanding Monomers: Synthesis, Characterization, and Applications. Boca Raton, Florida: CRC Press. ISBN 978-0-8493-5156-3.
* Nahrain E. Kamber; Wonhee Jeong; Robert M. Waymouth; Russell C. Pratt; Bas G. G. Lohmeijer; James L. Hedrick (2007). "Organocatalytic Ring-Opening Polymerization". Chemical Reviews. 107 (12): 5813–5840. doi:10.1021/cr068415b. PMID 17988157.
* Dubois, Philippe; Coulembier, Olivier; Raquez, Jean-Marie, eds. (2009). Handbook of Ring-Opening Polymerization. Wiley. doi:10.1002/9783527628407. ISBN 9783527628407.